Stock JCP V10
LIGHT-COLORED BROWN (KRAFT SHADE) ENVELOPES
Envelope February 1, 1999
Use information: This paragraph is informational only and is not exclusively definitive of the end use.
For the insertion of correspondences either manually or automated equipment. Suitable for letterpress and offset printing, processing
in laser printers, automated mail sorting equipment. Printed matter may include text and line illustrations.
Stock: 100 pct sulphate pulp. onds after sealing, the flap shall pull fibers from the body of the
Note: Not less than 20 pct postconsumer fiber. Any percent over envelope over the entire adhesive area.
20 percentage points is encouraged, provided that the require- The adhesive shall be able to resist the heat and pressure of
ments of this Standard are met. common office laser printers, so the flap adhesive does not be-
come soft and tacky causing the flap to stick to the body of the
Grammage (g/m2) ....................... 90 105 120 150 envelope.
Basis weight: 17 by 22 inches,
500 sheets (pounds) ................. 24 28 32 40 General appearance: Envelopes shall conform to the standard
sample(s) adopted by the Government.
A tolerance of ±5 pct shall be allowed.
Color: Shall be light-colored brown kraft shade. The envelopes
Bursting strength: Average, in the order shall be uniform.
not less than (kPa) ................... 260 300 340 410
Equivalent (lb/in2) .................... 38 44 50 60 Finish: Envelope stock shall have a smooth-finish.
Writing quality: Characters written with pen and ink shall be Cleanliness: The dirt count for each side of the paper shall not
clear cut and free from excessive feathering. exceed 250 specks per square meter. No envelope (up to
300 cm2 in size) shall contain no more than two obvious and ob-
Flap adhesive: The remoistenable adhesive on the sealing flaps jectionable with an equivalent area of 0.25 mm2 greater on the
of the envelopes shall have a minimum thickness of 0.015 mm face of the envelope. (The number of particles permitted is pro-
(0.0006 inch), uniformly applied. The flap shall not stick to the portionately higher for larger envelopes.)
body of the envelope, but shall be capable of being quickly and
securely sealed using 2.3 kg (5 pounds) pressure after moisten- Sampling and testing: Shall be conducted in accordance with
ing. When opened not less than 15 seconds or more than 20 sec- standards in Part 2, Government Paper Specification Standards.
Unless otherwise specified, the following is automatically waived when printing or duplicating is to be accomplished on commercial contract
Construction: Shall be specified by the ordering agency. (See Pressroom conditions: The bulk of these envelopes will be used
drawings in Part 3.) in air-conditioned pressrooms maintained at 24 ±2 °C and 45
Size: The size of the envelope shall be as ordered. A tolerance of ±8 pct relative humidity or offices with atmospheric conditions
¥2 mm, +4 mm shall be allowed. Dimensions are inside meas- of 21 ±5.5 °C and 50 ±20 pct relative humidity.